UV initiated thiol – ene chemistry : a facile and modular synthetic methodology for the construction of functional 3 D networks with tunable properties †

A facile methodology for the fabrication of functional crosslinked three dimensional (3D) networks has herein been explored via the benign and UV initiated thiol–ene coupling (TEC) chemistry. The careful selection of monomers or polymers and their feed ratio resulted in straightforward design of organic, inorganic and hydrogel networkswith readily available alkenes or thiol functional groups. All crosslinked networks were fabricated within 1 second of UV exposure at wavelengths of 320–390 nm and generally exhibited excellent gel fractions around 90%. By introducing off-stoichiometric thiol and ene (OSTE) monomer feed ratios the window of mechanical properties could bemanipulated. For the organic triazine system, the Young's modulus was altered from 780 MPa at an equimolar monomer ratio to soft 106 kPa for 2.5 equiv. with excess of thiol compared to enes. Postfunctionalizations with hydrophilic polyethylene glycols or acrylic acid and hydrophobic heneicosafluorododecyl acrylate were explored for the manipulation of functional networks. In this case, the rigid networks with excess of thiols were used as model substrates of which the initial contact angle (CA) of 60 was decreased to 43 by the introduction of acrylic acid and increased to 140 by successful attachment of fluorinated molecules. Finally, amalgamating micropatterning strategy with simple postfunctionalizations of hydrophobic groups resulted in superhydrophobic rigid surfaces with a CA of 173 .

The understanding of cell activities and behaviors in solution or on substrates is paramount for application driven research in therapeutic and diagnostic elds.For reasonable and accurate investigations of cell interaction mechanisms, the design of tunable 3D networks plays today an important role.In sensing applications, high detection resolution is strongly coupled to the optimization of the number of surface recognition sites and selectivity. 1From an accessibility point of view, the fabricated networks are preferably produced from commercial sources coupled with easy handling and excellent storage properties.Another important aspect is the mechanical properties of the networks, which allow enhanced cell adhesion. 2rosslinked 3D networks with readily available functionalities for facile postfunctionalizations deliver an elegant modular alternative to explore for biological studies.The ability to topographically functionalize such surfaces with anticipated substituents allows their use in an array of desired applications.For instance, covalent attachment of hydrophilic and/or biological sensing molecules enables the assessment of 3D networks in immunoassay and bio-recognition applications or as molecular imprinted networks. 3Additionally, in a number of biological studies in which small capillary channels are used as devices, the Young's modulus (E) window of the networks needs to be low enough for microfabrication but sufficiently high to maintain the geometry during low pressure operations.Typically, for PDMS networks the Young's modulus range is between 0.5 MPa and 5 MPa. 4,5However, in cell culture, so surfaces with a low modulus are preferable for efficient cell adhesion. 2onsequently, novel materials with tuneable modulus and programmable functionalities are continuously in demand in these elds.
Commonly, microarrays for biological studies and sensing applications are fabricated using commercial polydimethylsiloxane (PDMS) (Sylgard 184). 6Even though PDMS is robust and widely used, there are several limitations including (i) long thermal curing processes, 7 (ii) inherent hydrophobic nature, 6,8 (iii) chemical inertness in which plasmarization is required to introduce short-term hydrophilicity 9,10 and hydroxyl functional groups for further chemical modication, 7,8 and (iv) the geometry deformation which occurs under low pressure operation due to the low modulus. 11Considering the number of criteria of functional surfaces, a modular approach is herein exploited using UV initiated thiol-ene coupling (TEC) chemistry for the construction of functional 3D networks.The TEC chemistry has been extensively used due to the straightforwardness, robustness and the possibility to obtain high conversion, homogenous networks under ambient conditions and in the presence of oxygen. 12,13In contrast to the typical strategies relying on stoichiometrically balanced component ratios, for the development of neutral networks with maximized mechanical properties, the proposed methodology capitalizes on the off-stoichiometric ratio between thiol and ene (OSTE) monomers or polymers hence generating crosslinked functional 3D scaffolds with reactive sites available for further chemical modication. 14ubsequently, we demonstrate the construction of imbalanced 3D networks via TEC chemistry covering a wide range of modulus and based on organic and inorganic compounds in the form of three different network platforms each possessing unique properties.The monomer/polymer feed ratios as well as a selection of properties for these networks are detailed in Fig. 1 and Table 1.The rst set of networks were fabricated using triallyltriazinetrione (TTT) (1) and tris[2-(3-mercaptopropionyloxy)ethyl]isocyanurate (TMI) (2) as monomers.Six highly crosslinked networks with great stiffness, R1-R6, were obtained.In contrast to the rigid systems, the fabrication of so functional networks that were inherently hydrophilic or hydrophobic was also sought out.In the second network, by mixing allyl functionalized hydrophilic polyethylene glycol (PEG 3 kDa) (3) with a pentaerythritol tetraki-mercaptopropionate (PTM) (4) crosslinker at 33 wt% solids in ethanol, highly covalently crosslinked hydrogels exhibiting high water swelling capacity were successfully fabricated.For both the rigid triazine and hydrogel systems, 0.58 wt% of 2,2-dimethoxy-2-phenylacetophenone (DMPA) was used as a photoinitiator.So hydrophobic PDMS networks with high exibility and ductility were fabricated from vinyldimethylsiloxy terminated polydimethylsiloxane (5) (molecular weight ¼ 28 000 g mol À1 ) and poly(mercaptopropyl) methylsiloxane ( 6) (molecular weight ¼ 4000-7000 g mol À1 ) without the presence of photoinitiator.In all cases, the 3D networks were accomplished within 0.5 second total UV exposure at wavelengths of 320-390 nm and an intensity of 184 mW cm À2 .To investigate the network formation and the presence of unreacted functional groups, Fourier Transform RAMAN Spectroscopy (FT-RAMAN) was performed on a series of rigid networks.The spectra revealed C]C stretching at 1656 cm À1 representing excess reactive allyl groups (R1 and R2) and S-H stretching at 2564 cm À1 representing excess reactive thiol groups (R4-R6) (Fig. 2).Notably, network R3 with a balanced stoichiometric ratio of allyls to thiols displayed full consumption of both reactive groups.FT-RAMAN evaluation of excess functional groups on both hydrogel and PDMS 3D networks was uninformative due to the low end group concentration in comparison to the chain length of the prepolymers.To visualize the controlled introduction of available thiol groups, all the networks were corroborated by exploiting allyloxy disperse red 13 (7) as a visual colorimetric reagent. 15UV initiated postfunctionalization via thiol-ene click reactions 16,17 of networks with surplus of thiols resulted in increased covalent attachment of the colorimetric reagent.As shown in Fig. 3, the increased excess of available thiols within the lms resulted in higher degree of disperse red attachment which subsequently yielded stronger colouring outcome.Additionally, to quantify the available thiol groups aer lm formation, the networks were initially exposed to Ellman's reagent (5,5 0 -dithiobis-2nitrobenzoic acid (DTNB)) in phosphate buffer solution, pH 7. 18,19 The reagent selectively reacts with thiol groups forming the yellow chromophore derivative, 5-thio-2-nitrobenzoic acid (TNB), which possesses high absorbance at 412 nm.UV/vis analysis of TNB enables the determination of available thiols according to the absorbance calibration curve. 18The number of thiol molecules per cubic nanometer in hydrogel networks can be calculated by swelling hydrogels in DTNB solution.The hydrogel with balanced stoichiometric ratio H1 was found to include unreacted thiols of 0.019 molecules per nm 3 while H2 with a 2 : 1 ratio of [SH] : [allyl] revealed increased thiol active sites of 0.031 and 0.015 molecules per nm 3 for the network with excess of allyl H3 with a 1.5 : 1 ratio of [allyl] : [SH].As shown in Fig. 3, the presence of unreacted thiol groups in hydrogel network H1 was corroborated by the colorimetric reagent (7).H1 and H3 revealed the available thiol groups even though they are designed based on the equimolar feed ratio and excess of allyl.This is probably due to the restriction from an allyl PEG chain entanglement under the lm formation conditions which  hinder the probability of the reaction of all allyl groups leading to some unreacted thiols.
Unfortunately, the sensitivity of thiol detection through Ellman's reagent was found insufficient for both rigid and so inorganic networks.In this case, the limited network swelling with aqueous Ellman's solution results in unsuccessful interactions with excess thiols.Moreover, due to the hydrophobic nature and high mobility of the silicon networks, the thiol groups can be shielded for further reactions with the reagent under aqueous conditions.As seen in Table 1 and Fig. 4, the mechanical properties were controlled by altering both the composition of the components as well as the feed ratio between thiol and ene.For the rigid systems, the network with balance ratio R3 displayed the highest crosslinking density with a gel fraction close to 100%, an average molecular weight between a crosslink M c of 800 g mol À1 and Young's modulus with a value above 780 MPa.The introduction of the off-stoichiometric strategy with unreacted functional groups resulted in looser networks with a higher value of M c .Interestingly, a direct comparison between networks with excess of allyl or thiol with the same off stoichiometric ratio (R2 vs. R4) revealed similar gel fractions of 98% but with a lower E value and higher M c for the networks with excess of thiol.In this case, the excess of allyl groups in R2 resulted in Young's modulus value of 615 MPa and a M c of 900 g mol À1 while excess of thiol in R4 noted a Young's modulus value of 89 MPa and M c of 1700 g mol À1 .The apparent drop in mechanical properties may be due to the more exible structure of the triazine thiol monomer or consumption of thiols forming spontaneous disulphide cyclization that does not participate during the crosslinking process.Moreover, the more rigid systems achieved for R2 can be a consequence of homo-crosslinking between the available allyls.It should be noted that the homopolymerization of triallyltriazinetrione (1) using similar conditions as thiol-ene networks resulted in viscous gel with a gel fraction of 2.6%.Additional increase of thiols resulted in lower gel fractions reaching 68% at 2.5 molar ratio excess (R6).Notably, the obtained organic gels were found so and loosely crosslinked, similar to the mechanical properties of commercially available inorganic PDMS networks, and with a Young's modulus value of 106 kPa and M c of 31 000 g mol À1 .In the case of so networks, the inorganic system S2 shows the lowest M c of 12 000 g mol À1 and swelling degree in chloroform as well as the highest gel fraction of 89% and Young's modulus of 266 kPa.
For hydrogels, both the balance ratio (H1) and excess of thiol (H2) have similar swelling/leaching properties in water compared to excess of allyl (H3) which can be seen from H3's lower gel fraction.Young's modulus and values of M c estimated from stiffness properties of the hydrogel network are practically similar.Satised with the modular strategy that delivers functional surfaces covering a range of modulus, the lms were further exploited as templating scaffolds to manipulate their nal properties by facile chemical modications of readily available functional groups.In this context, the available thiols were approached for postfunctionalization purposes as these can efficiently react with a number of complementary reactive Fig. 3 Postfunctionalization with a visual colorimetric reagent allyloxy disperse red 13 (7) with increasing thiol surplus.groups including alkenes and alkynes, nucleophilic addition to epoxies and isocyanates, or through Michael addition. 20ollowing a similar solution based modication strategy as for the attachment of the colorimetric reagent (7) i.e. the robust and UV-initiated TEC click reaction, 17 the substrates were conceptually postfunctionalized to deliver hydrophilic surfaces using acrylic acid (8), acrylamide (9) and allyloxy polyethylene glycol (11) as well as hydrophobicity by the attachment of the uorinated compound, heneicosauorododecyl acrylate (10).
While the functionalizations of the rigid networks were topological, the so inorganic and hydrogel networks were homogenously modied.The latter was accomplished by swelling the networks in a mixture of reactive vinylic molecules and catalytic amounts of DMPA and followed by UV initiated TEC reactions.For the rigid substrates, R5 based on the 1.9 offstoichiometric amount of thiols was chosen as a scaffolding surface due to the moderate amount of unreacted thiol and robust mechanical properties.As can be seen in Fig. 5, the initial contact angle (CA) for the R5 lm was noted at 60 .Aer surface modications with a solution of acrylic acid (8) or allyloxy PEG (11), at UV exposure less than 1 second with a dosage of 372 mJ cm À2 , followed by thorough washing procedures, the lms displayed increased wettability with a contact angle decrease to 43 and 52 , respectively.To alter the surface properties to exhibit hydrophobicity, heneicosauorododecyl acrylate (10) was allowed to react with the R5 lm which resulted in an increase of 80 to a CA of 140 .For the so hydrogels and inorganic systems, acrylic acid (8) and acrylamide (9) were efficiently attached to H2 and S3 networks.Aer solvent wash of the crosslinked system, FT-IR spectra (ESI S4 and S5 †) showed the presence of N-H stretching at 1608 cm À1 and C]O at 1666 cm À1 for the acrylamide substituent.Similarly, the attachment of acrylic acid for the so PDMS network shows the C]O stretching at 1711 cm À1 as well as an increased peak for the hydrogel C]O stretching when compared to the reference PEG network.In the case of so PDMS based networks, the contact angle measurements did not display any decrease.This is due to the mobility of PDMS that migrates from the bulk to the surface resulting in hydrophobic recovery. 9Nonetheless, the attachment of the colorimetric reagent (7) resulted in a strong visual signal corroborating successful covalent postfunctionalization (Fig. 3).To further expand on the feasibility of the proposed methodology, microfabrication via the moulding technique 21 was utilized to generate functional surfaces with increased topographic roughness and hydrophobicity. 22n attractive eld of research capitalizes on superhydrophobic substrates that exhibit repelling properties with CA around 150 that are in need in numbers of applications.Such surfaces nd use as self-cleaning paints and textiles 22 and in emerging applications such as DNA microarrays requiring specic wetting of the substrate. 22Both rigid (R5) and so (S3) networks were patterned utilizing submicron ridge/groove silicon master structures (10 mm), ESI Fig. S6.† The effect of surface topology raises the CA for the PDMS substrates (S3) from 120 to superhydrophobic 149 (Fig. 6a and b).Increasing the roughness on rigid networks (R5) resulted in an increase of CA to 120 (Fig. 6c and d).Remarkably, amalgamating surface patterning of the rigid thiol functional substrate (R5) and postfunctionalization procedures with heneicosauorododecyl acrylate (10) resulted in the superhydrophobic surface that displayed a static CA of 173 based on 10 ml water droplets (Fig. 6e).In fact, due to strong repulsion forces the contact angle measurements with water droplets of 5 ml were fruitless.As can be seen in Fig. 6f, a 8 second picture sequence showcases the superhydrophobicity making these surfaces ideal as water repellent rigid substrates (see video S1 † for the superhydrophobic water repellence surface with 5 and 10 ml water droplets).
In summary, we herein describe a modular approach that exploits the highly efficient and UV initiated thiol-ene coupling chemistry for the fabrication of functional network templates with controllable mechanical properties.By carefully choosing the components and their off-stoichiometric feed, thiol and allyl, functional 3D networks were efficiently constructed under less than 1 second UV exposure at wavelengths of 320-390 nm.The window of Young's modulus obtained ranges from 780 MPa for rigid organic networks to 18 kPa for hydrogel systems.The fabricated networks were further utilized as reactive templates for the functionalization with several vinylic molecules including colorimetric agent to visually conrm successful covalent attachment to the readily available thiol groups.Additionally, the wettability of the networks was manipulated by the introduction of hydrophilic compounds such as PEGallylated chains and hydrophobic uorinated groups.The introduction of surface roughness through microfabrication coupled with facile postfunctionalizations of uorinated substituents increased the contact angle of a rigid organic substrate from 60 to superhydrophobic 173 .

Fig. 1
Fig. 1 Schematic representation of three different functional networks and the postfunctionalization molecules.

Fig. 4
Fig.4Young's modulus of the functional network at room temperature (25 C).

Fig. 6
Fig. 6 The effects of surface roughness and postfunctionalization on functional surfaces shown by contact angle measurements and SEM images.(a and b) Flat and structured soft PDMS network S3; (c and d) flat and structured rigid organic network R5; (e) facile postfunctionalization of R5 to obtain superhydrophobic surface properties; (f) 1 second snapshots of water rejection of the superhydrophobic substrate.

Table 1
Mechanical properties of functional networks with a series of stoichiometric ratios M c was calculated from DMTA (rigid and so networks) and swelling properties (hydrogel network).b Swelling tests were performed in acetone (rigid network), water (hydrogel network) and chloroform (so network). a